INTERNATIONAL JOURNAL OF RESEARCH IN TECHNOLOGY (IJRT) Vol. V, No. III, June 2018

ISSN No. 2394-9007 www.ijrtonline.org

Heats of Absorption on the Catalytic Surfaces of Organic Molecules Anupama Sharma

This could be measured with the help of micro calorimetery or other methods. In order to understand this phenomenon of adsorption, activation and desorption a number of mathematical models have been proposed soon after the proposal of Langmuir adsorption theory7. During recent days a number of quantum theoretical methods like Mont Carlo simulation and ab initio methods and applied for complicated system of hydrocarbons as well as amino acid to model the system of interest8. In this paper we have follow a simple approach for predicting the heat of adsorption taking the case of pentane over two different surfaces ZSM-5 or Silicalite whose most general MFI structure shown in Fig 1-2. ZSM-5 (MFI topology) is a very important zeolite and is widely used as shape-selective catalysts in industry.

Abstract—When the molecules is absorbed on the interacting surfaces of organic molecules the phenomenon is called adsorption. The number of chemical reactions proceed by the phenomenon of adsorption of organic molecules the heat is liberated which is called the heat of adsorption and this can be calculated by using the mathematical chemistry and gauss Bonett Theory differential geometry. The physico-chemical properties of organic molecules depend on the nature of catalytic surfaces of organic molecules. The importance of this methods used in the study of bio-chemical reaction and catalytic reaction proceed on the surfaces of organic molecules. Keywords: Jeolites.

I. INTRODUCTION Adsorption is the net accumulation of a chemical species at the interface between a solid phase and an aqueous solution phase, leading to a loss from the solution phase. It plays a significant role in catalytic reactions like isomerisation, oligomerisation, alkylation and cracking of hydrocarbons and many more processes like adsorptive separations of isomers3. The study of adsorption energies (Heats of adsorption DH) on such system provides strength of adsorbate surface. As such adsorption is a surface phenomenon. Most of the study reported so far may be classified into three groups. Firstly, those which deal with adsorption of molecules on metal surfaces, secondly the adsorption of hydrocarbons of materials like surfaces of zeolites, clay and hetropoly acids and thirdly those which deal with the adsorption of proteins on solids and are responsible in biochemical reactions.

The curvature of surfaces of ZSM-5 and silicalite were calculated with the help of Gauss-Bonett theorem as describe by ANDERSSON. The Gauss Bonett Theorem reads as follows: Using the numerical integration of the Weierstras equation one can easily calculate the cartesian coordinates and Gaussian curvatures of the D. P and G surfaces. It dA is the area of a surface element S and dA’ is the Gauss map S* of S, then : Thus òòdAs = òòS* Kdsd A’/K 1

II. SURFACE

IV. STRUCTURE OF ZEOLITE ZSM-5 AND SILICALITE

III. EXPERIMENTAL AND THEORETICAL DETAILS AND METHODS

Mathematically, a surface is defined as Z = f(x,y) and its curvature is defined by Gauss Bonnet theorem6. In catalysis and biochemical reactions like adsorption of protein and hydrocarbons takes place on such surfaces. Under suitable conditions these molecules are activated and reach to a transition state and finally adopt a suitable pathway of transformation by desorption. This molecular process is terminated after liberating some heat called heat of adsorption (DH). Manuscript received on June, 2018. Dr. Anupama Sharma, Applied Science, Shiwalik College of Engineering, Dehradun, Himachal Pradesh, India. Fig. 1: Structure of ZEOLITE ZSM-5 and SLICALITE

Impact Factor: 4.012 Published under Asian Research & Training Publication ISO 9001:2015 Certified

65

INTERNATIONAL JOURNAL OF RESEARCH IN TECHNOLOGY (IJRT) Vol. V, No. III, June 2018 V. HEAT OF ABSORPTION

ISSN No. 2394-9007 www.ijrtonline.org

VI. HEAT OF ABSORPTION OF HYDROCARBONS ON DIFFERENT ZEOLITE SURFACES

Where N is the bonding electron per molecule which scales very well with the average polarizabilities of hydrocarbons and S is surface constant. Hence a differential heat of adsorption: Can be calculated. By assuming that the adsorbateadsorbent interaction is very clean and the adsorbateadsorbate interaction is negligible. D H = S N.Kav 10 Where S is another interface constant considering the above facts it is worthwhile to quantify initial heat of adsorption. H in terms of the curvature of the catalyst surface the delta function polarizability ám of the interacting hydrocarbons and surface constant by the relation. D H = ám.â.ã+èf 11 In a recent work, the study has been extended to hydrocarbons. Having deciphered the values of the heats of adsorption the activation energy E has been verified by Evans-Polyani method to explain the reaction rates. Inside a zeolite molecule should feel an attractive force F F = Constant. N .Kav 12 On the Basis these workers (19) verified the measurement of Stach.ET.AL (13, 19) on the heat of adsorption of hydrocarbons on different Zeolites. Considering above observe facts, it is worth to quantify initial heat of adsorption D H in terms of curvature of zeolite surface = Kav, the delta function polarizability ám of interacting hydrocarbons.

120 100 80 60 40 20 0 1

HZSM-5

Faujasite

Silicalite

Mordenite

2

3 4 5 6 Carbon Number of Alkanes

7

8

Fig.3: Trends of Heats of Adsorption of n-alkanes on Different Zeolite Surfaces as a Function of their Carbon Number

Fig. 3: Trends of Heats of Absorption of n-alkanes on different

VII. OBSERVATIONS & RESULTS The curvature of ZSM – 5 and silicalite calculated on the basis of differential geometry and Gauss Bonett theorem has been found to be – 0.065A and - .0584A The heat of adsorption on these two surfaces is found to be 14.82 on ZSM- 5 and 15.15–A on silcalite surfaces respectively. The experimental values obtained by Stach, Fiedler and Janchen are 14.35 kilo calorie/mole. This value matches very closely with our theoretical results showing the basic soundness of the method adopted. Taking the advantage of this calculation, the heats of adsorption for alkanes on mordenite and faujasite has been calculated and displayed in Fig3. VIII. DISCUSSION The area of surface contained in one unit cell of the dealuminated faujasite structure of unit cell a = 24.20 Å becomes 2261 Å2 and a tetrahedral saddle 47.11 Å2. and the average curvature is: Kav = -2/3. p / 47.11 = - 0.0445 Å2. This equation was now tested by using accurate adsorption heats of hydrocarbons in estimating the surface curvature of mordenite, silicalite, and ZSM-5 that was found to be 0.04, -0.05 and -0.03Å respectively. The heats of adsorption data8 for paraffins, naphthenes, aromatic, olefins on different zeolites surfaces were computed using the above curvature data and their polarizabilities. The data on heats of adsorption shows fair degree of agreement with the experimental values. Only the representative data on adsorption and activation energy of n-alkanes ZSM-5 system have been collected and displayed in Fig 3 * The detailed account of adsorption data of hydrocarbons on zeolite surfaces are available to justify a method of calculation but taking the case of pentane, that absorbs on ZSM -5 and silicalite gives different values of D H although the value of content is the same meaning thereby the surface quantity curvature plays a significant role in adsorption phenomenon this is the reason why the same hydrocarbon species adsorb on two different surfaces

Fig. 2: Heat of Absorption

Impact Factor: 4.012 Published under Asian Research & Training Publication ISO 9001:2015 Certified

66

INTERNATIONAL JOURNAL OF RESEARCH IN TECHNOLOGY (IJRT) Vol. V, No. III, June 2018 [2]

possess different heat of adsorption and hence different rates of chemical reaction. The heats of adsorption of n-alkanes are proportional to the curvature of ZSM-5 surface and vary as the product of surface curvature and the electric polarizabilities of nparaffins. This observation is in line with similar increase with carbon number or chain length with a difference that our treatment is based on the cooperative effect between absorbate and substrate and explains clearly why heats of adsorption of the same alkane interacting with different zeolities should possess different DH values.

D.B. and H K Christenson, J. Phys. Chem. Vol 96, p 3395, 1992

[3] Silva, J.A.C.; Rodrigues, A.E. Industrial and Engineering Chemistry Research ; VOL. 36 ; ISSUE: 2 ; PBD: Feb 1997 [4]

Deyaner F. M., Souverikan W., Jacob P. A., Matins J. A. and Baron G. V., J. Phys. Chem., 102, 4588-4597, (1998).

[5]

P. Magnoux, Y. Boucheffa, M. Guisne, G. Joly and S. Jullian Oil & Gas Science and Technology – Rev. IFP, Vol. 55 (2000), No. 3 p 308

[6] Andersson S., Angew Chem., 22, 69-170, (1983) Langmuir, I. JACS, 38, 2221. 1916 [7] Dixit Lalji and Prasad Rao T S R, Recent Trends in 9.Catalysts, Narosa Publishing House, New Delhi, 1999.

REFERENCES [1] Chen N. Y., Garwood W. E. and Dwyer F. G., Shape Selective Catalyst in Industrial Applications, 2nd Ed. Marcel Dekker, N Y 1996.

Impact Factor: 4.012 Published under Asian Research & Training Publication ISO 9001:2015 Certified

ISSN No. 2394-9007 www.ijrtonline.org

[8]

Hyde H. T., Acta. Chem. Scand., 45, 860-863, (1993).

[9] Andersson S., Angew Chem., 22, 69-170, (1983).

67

Heats of Absorption on the Catalytic Surfaces of Organic Molecules

When the molecules is absorbed on the interacting surfaces of organic molecules the phenomenon is called adsorption. The number of chemical...

Heats of Absorption on the Catalytic Surfaces of Organic Molecules

Published on Jul 13, 2018

When the molecules is absorbed on the interacting surfaces of organic molecules the phenomenon is called adsorption. The number of chemical...

Advertisement